Spreadsheet: 5252cd43-8925-4b22-b22c-2308f6214aa8
Sheet: Sheet1

Comparative Physical Properties of Popular Wood Species
Species | Specific Gravity† | Weight‡ | Strength | Stiffness | Hardness | Shock Resisting Ability | [NAME] | Shrinkage
ALDER, RED | 0.37 | 28 | 82 | 139 | 48 | 71 | 76 | 123
ASH, WHITE | 0.54 | 41 | 106 | 161 | 108 | 139 | 110 | 126
ASPEN | 0.35 | 27 | 58 | 107 | 31 | 67 | 63 | 111
AVODIRE |  | 36 | 97 | 125 | 93 | 81 | 96 | 105
BASSWOOD | 0.32 | 26 | 62 | 126 | 31 | 54 | 61 | 158
BEECH | 0.56 | 45 | 94 | 169 | 96 | 135 | 102 | 162
BIRCH, [NAME] | 0.6 | 46 | 105 | 207 | 104 | 159 | 117 | 154
BIRCH, YELLOW | 0.55 | 43 | 98 | 174 | 86 | 171 | 106 | 166
[NAME] |  | 55 |  |  | 157 |  |  | 148
BUTTERNUT | 0.36 | 27 | 68 | 115 | 40 | 80 | 64 | 100
CATALPA, NORTHERN | 0.38 | 29 | 59 | 110 | 43 | 95 | 63 | 73
CATIVO | 0.4 | 29 | 60 | 101 | 50 | 60 | 68 | 85
CHERRY, BLACK | 0.47 | 35 | 100 | 150 | 72 | 112 | 93 | 113
CHESTNUT | 0.4 | 30 | 70 | 112 | 50 | 69 | 68 | 111
COTTONWOOD, EASTERN | 0.37 | 28 | 64 | 123 | 36 | 73 | 62 | 138
CUCUMBER TREE, YELLOW | 0.44 | 34 | 88 | 175 | 57 | 103 | 90 | 137
CYPRESS, BALD | 0.42 | 32 | 92 | 136 | 52 | 76 | 79 | 104
DOGWOOD | 0.64 | 51 | 101 | 124 | 154 | 192 | 100 | 194
EBONY |  | 63 | 174 | 230 | 258 | 255 | 196
ELM, AMERICAN | 0.46 | 36 | 74 | 130 | 66 | 123 | 85 | 145
HACKENBERRY | 0.49 | 37 | 72 | 108 | 74 | 145 | 76 | 138
HICKORIES, TRUE | 0.65 | 51 | 123 | 188 | 142 | 292 | 138 | 182
HOLLY | 0.5 | 40 | 71 | 102 | 86 | 124 | 76 | 155
LIMBA | 0.45 | 34 | 73 | 101 | 70 |  | 28 | 140
LOCUST, BLACK | 0.66 | 48 | 168 | 220 | 161 | 170 | 157 | 103
MAHOGANY, AFRICAN | 0.43 | 31 | 91 | 104 | 68 | 80 | 87 | 92
MAHOGANY, CENTRAL AMERICA | 0.45 | 32 | 111 | 145 | 76 | 83 | 98 | 79
MAHOGANY, CUBAN | 0.57 | 41 | 95 | 123 | 114 | 71 | 88 | 60
MAKORE |  | 40 |  |  |  |  |  | 124
MAPLE, RED | 0.49 | 38 | 87 | 158 | 79 | 110 | 93 | 128
MAPLE, SILVER | 0.44 | 33 | 71 | 106 | 65 | 93 | 69 | 114
MAPLE, SUGAR | 0.57 | 44 | 106 | 178 | 115 | 138 | 114 | 147
MERANTI, RED (LAUAN) | 0.4 | 36 | 86 | 138 | 55 | 110 | 82 | 117
MERANTI, WHITE (LAUAN) |  | 36 | 75 | 138 | 53 | 114 | 74 | 103
MYRTLE | 0.51 | 39 | 76 | 89 | 106 | 144 | 72 | 116
NARRA | 0.52 | 42 | 148 | 159 | 124 | 149 | 136 | 69
OAKS, COMMERCIAL RED | 0.56 | 44 | 92 | 168 | 103 | 139 | 101 | 143
OAKS, COMMERCIAL WHITE | 0.59 | 47 | 93 | 149 | 109 | 125 | 99 | 155
ORIENTALWOOD |  | 44 | 122 | 150 | 117 |  | 105
OSAGE-ORANGE | 0.76 |  | 147 | 153 | 246 | 397 | 157 | 89
PADAUK (AFRICAN) |  | 43 |  |  | 137 |  |  | 82
PADAUK (ANDAMAN) | 0.62 | 45 | 152 | 165 | 130 | 101 | 130 | 78
PADAUK (BURMA) | 0.75 | 54 | 187 | 196 | 198 | 159 | 176
PALDAO | 0.54 | 44 |  |  | 94 |  |  | 127
PEARWOOD (EUROPEAN) |  | 43 |  |  | 94 |  |  | 195
PECAN | 0.6 | 47 | 104 | 162 | 142 | 156 | 110 | 137
PRIMAVERA | 0.4 | 30 | 102 | 123 | 74 | 94 | 106 | 91
ROSEWOOD (BRAZIL) |  | 50 |  |  | 153 |  |  | 119
SAPELE | 0.54 | 40 | 137 | 126 | 123 | 94 | 96 | 138
SATINWOOD | 0.83 | 67 | 166 | 181 | 209 | 132 | 141 | 147
SONORA (MANNGGASINORO) | 0.42 | 31 | 62 | 116 | 50 | 88 | 61
SWEETGUM | 0.44 | 34 | 77 | 134 | 60 | 99 | 86 | 150
SYCAMORE | 0.46 | 35 | 76 | 129 | 64 | 78 | 74 | 136
TANGUILE | 0.53 | 39 | 91 | 154 | 64 | 87 | 87 | 103
TEAK | 0.6 | 43 | 136 | 173 | 99 | 107 | 124 | 162
TIGERWOOD | 0.45 | 34 | 101 | 123 | 78 | 93 | 90 | 138
TULIPWOOD, AMERICAN | 0.38 | 28 | 68 | 135 | 40 | 58 | 71 | 119
TUPELO, WATER | 0.46 | 35 | 87 | 127 | 78 | 81 | 82 | 122
WALNUT, BLACK (AMERICAN) | 0.51 | 39 | 113 | 167 | 88 | 124 | 111 | 116
WILLOW, BLACK | 0.34 | 26 | 41 | 70 | 35 | 91 | 45 | 126
ZEBRAWOOD | 0.62 | 48 |  |  | 125 |  |  | 156